Loading in 2 Seconds...
Loading in 2 Seconds...
University of Waterloo Department of Mechanical Engineering ME 322  Mechanical Design 1 Partial notes – Part 4 (Fatigue) (G. Glinka) Fall 2005. N i = ? N p = ? N T = ?.
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Department of Mechanical Engineering
ME 322  Mechanical Design 1
Partial notes – Part 4 (Fatigue)
(G. Glinka)
Fall 2005
Np = ?
NT = ?
Metal Fatigueis a process which causes premature irreversible damage or failure of a component subjected to repeated loading.
FATIGUE  What is it?
Fatigue is not cause of failure per se but leads to the final fracture event.
(from Ewalds & Wanhil, ref.3)
Δσ
Δσ
Schematic of Fatigue Crack Initiation Subsequent Growth Corresponding and Transition From Mode II to Mode ILocally, the crack grows in shear;
macroscopically it grows in tension.
A – fatigue crack area
B – area of the final static failure
(Collins, ref. 22 )
Applied Stresses
Materials
History
Material
Properties
Component
Geometry
StressStrain
Analysis
Damage
Analysis
Allowable Load  Fatigue Life
StrengthFatigue Analysis ProcedureInformation path in strength and fatigue life prediction procedures
speak
Stress
a)
n
S
r
y
0
speak
Stress
dn
n
T
r
0
y
dn
T
Stress Parameters Used in Static Strength and Fatigue Analysesb)
S
Constant amplitude stress history
max
In the case of the peak stress history the important parameters are:
m
Stress
One cycle
min
0
Time
Variable amplitude stress history
b)
Stress
One reversal
Time
0
Constant and Variable Amplitude Stress Histories;Definition of a Stress Cycle & Stress ReversalStress history
i+1
Stress
i1
i2
i+2
Time
i
Stress History and the “Rainflow” Counted CyclesA rainflow counted cycle is identified when any two adjacent reversals in thee stress history satisfy the following relation:
A rainflow counted cycle is identified when any two adjacent reversals in thee stress history satisfy the following relation:
The stress amplitude of such a cycle is:
The stress range of such a cycle is:
The mean stress of such a cycle is:
The Mathematics of the Cycle Rainflow Counting Method for Fatigue Analysis of Stress/Load Histories6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
Reversal point No.
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
Reversal point No.
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
Reversal point No.
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
6
5
4
2
3
2
Stress (MPa)x10
1
0
0
1
2
3
4
5
6
7
8
9
10
11
12
13
14
1
2
3
Reversal point No.
Number of Cycles According to the Rainflow Counting Procedure (N. Dowling, ref. 2)
Note! In the case of smooth components such as the railway axle the nominal stress and the local peak stress are the same!
B
A
Smin
Smax
Wöhler’s Fatigue TestPart 1
Part 2
Part 3
Fatigue SN curve
Su
S103
Sy
Stress amplitude, Sa (ksi)
Se
Number of cycles, N
Fully reversed axial SN curve for AISI 4130 steel. Note the break at the LCF/HCF transition and the endurance limit
Characteristic parameters of the S  N curve are:
Se  fatigue limit corresponding to N = 1 or 2106 cycles for
steels and N = 108 cycles for aluminum alloys,
S103  fully reversed stress amplitude corresponding to N = 103
cycles
m  slope of the high cycle regime curve (Part 2)
Most of available S  N fatigue data has been obtained from fully reversed rotational bending tests. However, material behavior and the resultant S  N curves are different for different types of loading. It concerns in particular the fatigue limit Se.
S103
Se
1.0
0.5
Relative stress amplitude, Sa/Su
Bending
Axial
0.3
Torsion
0.1
105
104
106
107
103
Number of cycles, Log(N)
The stress endurance limit, Se,of steels (at 106 cycles) and the fatigue strength, S103 corresponding to 103 cycles for three types of loading can be approximated as (ref. 1, 23, 24):
S103 = 0.90Su and Se = S106 = 0.5 Su  bending
S103 = 0.75Su and Se = S106 = 0.35  0.45Su  axial
S103 = 0.72Su and Se = S106 = 0.29 Su torsion
Approximate endurance limit for various materials:
Magnesium alloys (at 108 cycles) Se = 0.35Su
Copper alloys (at 108 cycles) 0.25Su< Se <0.50Su
Nickel alloys (at 108 cycles) 0.35Su <Se < 0.50Su
Titanium alloys (at 107 cycles) 0.45Su <Se< 0.65Su
Al alloys (at 5x108 cycles) Se = 0.45Su (if Su ≤ 48 ksi) or Se = 19 ksi (if Su> 48 ksi)
Steels (at 106 cycles) Se = 0.5Su (if Su ≤ 200 ksi) or Se = 100 ksi (if Su>200 ksi)
Irons (at 106 cycles) Se = 0.4Su (if Su ≤ 60 ksi) or Se = 24 ksi (if Su> 60 ksi)
S – N curve
Fatigue Limit – Modifying Factors
For many years the emphasis of most fatigue testing was to gain an empirical understanding of the effects of various factors on the baseline SN curves for ferrous alloys in the intermediate to long life ranges. The variables investigated include:
 Rotational bending fatigue limit, Se’,
 Surface conditions, ka,
 Size, kb,
 Mode of loading, kc, Se = ka kb kc kd ke kf·Se’
 Temperature, kd
 Reliability factor, ke
 Miscellaneous effects (notch), kf
Fatigue limit of a machine part, Se
Surface Finish Effects on Fatigue Endurance Limit
The scratches, pits and machining marks on the surface of a material add stress concentrations to the ones already present due to component geometry. The correction factor for surface finish is sometimes presented on graphs that use a qualitative description of surface finish such as “polished” or “machined”.
Below a generalized empirical graph is shown which can be used to estimate the effect of surface finish in comparison with mirrorpolished specimens [Shigley (23), Juvinal (24), Bannantine (1) and other textbooks].
ka
Effect of various surface finishes on the fatigue limit of steel. Shown are values of the ka, the ratio of the fatigue limit to that for polished specimens.
Ca
(from J. Bannantine, ref.1)
Size Effects on Endurance Limit
0.95max
+
0.95d
0.05d/2
t

0.95t
F
The effective diameter, de, for members with noncircular cross sections
The material volume subjected to stresses 0.95max is concentrated in the ring of 0.05d/2 thick.
The surface area of such a ring is:
* rectangular cross section under bending
Equivalent diameter
Loading Effects on Endurance Limit
The ratio of endurance limits for a material found using axial and rotating bending tests ranges from 0.6 to 0.9.
The ratio of endurance limits found using torsion and rotating bending tests ranges from 0.5 to 0.6. A theoretical value obtained from von MisesHuberHencky failure criterion is been used as the most popular estimate.
From: Shigley and Mischke, Mechanical Engineering Design, 2001
The reliability factor accounts for the scatter of reference data such as the rotational bending fatigue limit Se’.
The estimation of the reliability factor is based on the assumption that the scatter can be approximated by the normal statistical probability density distribution.
The values of parameter za associated with various levels of reliability can be found in Table 77 in the textbook by Shigley et.al.
SN curves for assigned probability of failure; P  S  N curves
(source: S. Nishijima, ref. 39)
Stress concentration factor, Kt, and the notch factor effect, kf
Fatigue notch factor effect kf depends on the stress concentration factor Kt (geometry), scale and material properties and it is expressed in terms of the Fatigue Notch Factor Kf.
Similarities and differences between the stress field near the notch and in a smooth specimen
P
S
peak
Stress
n=S
peak= n=S
r
x
0
dn
W
The Notch Effect in Terms of the Nominal Stress
S
N (DS)m = C
n1
DSmax
S
n2
DS2
Sesmooth
n3
n4
Stress range
N2
N0
cycles
np
Fatigue notch factor!
Definition of the fatigue notch factor Kf
M
S
2
2
speak
s22= speak
Stress
Stress
Nsmooth
2
Se
1
1
1
3
Nnotched
Nnotched
a – constant,
r – notch tip radius;
NEUBER’s approach
ρ – constant,
r – notch tip radius
Curves of notch sensitivity index ‘q’ versus notch radius (McGraw Hill Book Co, from ref. 1)
Illustration of the notch/scale effect
Plate 1
W1 = 5.0 in
d1 = 0.5 in.
Su = 100 ksi
Kt = 2.7
q = 0.97
Kf1 = 2.65
peak
peak
m1
m2
d2
Plate 2
W2= 0.5 in
d2 = 0.5 i
Su = 100 ksi
Kt = 2.7
q = 0.78
Kf1 = 2.32
d1
W2
W1
Collins method
Juvinal/Shigley method
Nf (logartmic)
Sar, ar – nominal/local stress amplitude at zero mean stress m=0 (fully reversed cycle)!
Nf (logartmic)
Procedures for construction of approximate fully reversedSNcurves for smooth and notched componentsProcedures for construction of approximate fully reversedSNcurves for smooth and notched components
Manson method
0.9Su
Sar (logartmic)
Se’kakckbkdke
Se’kakckbkdkekf
Se
104
101
102
105
106
2·106
103
100
Nf (logartmic)
Sar, ar – nominal/local stress amplitude at zero mean stress m=0 (fully reversed cycle)!
Constant amplitude cyclic stress histories
Pulsating
m = a R = 0
Fully reversed
m = 0, R = 1
Cyclic
m > 0 R > 0
Stress amplitude, Sa
0
sm= 0
time
sm< 0
sm< 0
Stress amplitude, logSa
sm= 0
sm> 0
No. of cycles, logN
2*106
Mean Stress Effect
The tensile mean stress is in general detrimental while the compressive mean stress is beneficial or has negligible effect on the fatigue durability.
Because most of the S – N data used in analyses was produced under zero mean stress (R = 1) therefore it is necessary to translate cycles with non zero mean stress into equivalent cycles with zero mean stress producing the same fatigue life.
There are several empirical methods used in practice:
The Hiagh diagram was one of the first concepts where the mean stress effect could be accounted for. The procedure is based on a family of Sa – Sm curves obtained for various fatigue lives.
Steel AISI 4340,
Sy = 147 ksi(Collins)
Mean Stress Correction for Endurance Limit
Sa – stress amplitude applied at the mean stress Sm≠ 0 and fatigue life N = 12x106cycles.
Sm mean stress
Se fatigue limit at Sm=0
Su ultimate strength
f’ true stress at fracture
Gereber (1874)
Goodman (1899)
Soderberg (1930)
Morrow (1960)
Mean stress correction for arbitrary stress amplitude applied at nonzero mean stress
Sa – stress amplitude applied at the mean stress Sm≠ 0 and resulting in fatigue life of N cycles.
Sm mean stress
Sar fully reversed stress amplitude applied at mean stress Sm=0 and resulting in the same fatigue life of N cycles
Su ultimate strength
f’ true stress at fracture
Gereber (1874)
Goodman (1899)
Soderberg (1930)
Morrow (1960)
Comparison of various methods of accounting for the mean stress effect
Most of the experimental data lies between the Goodman and the yield line!
The following generalisations can be made when discussing mean stress effects:
1. The Söderberg method is very conservative and seldom used.
3. Actual test data tend to fall between the Goodman and Gerber curves.
3. For hard steels (i.e., brittle), where the ultimate strength approaches the true fracture stress, the Morrow and Goodman lines are essentially the same. For ductile steels (of > S,,) the Morrow line predicts less sensitivity to mean stress.
4. For most fatigue design situations, R < 1 (i.e., small mean stress in relation to alternating stress), there is little difference in the theories.
5. In the range where the theories show a large difference (i.e., R values approaching 1), there is little experimental data. In this region the yield criterion may set design limits.
6. The mean stress correction methods have been developed mainly for the cases of tensile mean stress.
For finitelife calculations the endurance limit in any of the equations can be replaced with a fully reversed alternating stress level corresponding to that finitelife value!
n
1
Ni(si)m = a
n
s2
2
s3
n
3
Stress range,
s
e
n
4
'
s
e
N1
N
N3
N
c
c
y
l
e
s
o
2
NT
Procedure for Fatigue Damage Calculation
n1  number of cycles of stress range1 n2  number of cycles of stress range2ni  number of cycles of stress rangei,
 damage induced by n1 cycles of stress range 1,
 damage induced by one cycle of stress range 1,
 damage induced by one cycle of stress range 2,
 damage induced by n2 cycles of stress range 2,
 damage induced by one cycle of stress range i,
 damage induced by ni cycles of stress range i,
Total Damage Induced by the Stress History
It is usually assumed that fatigue failure occurs when the cumulative damage exceeds some critical value such as D =1,
i.e. if D > 1  fatigue failure occurs!
For D < 1 we can determine the remaining fatigue life:
LR  number of repetitions of the stress history to failure
N  total number of cycles to failure
Results of "rainflow" counting
D a m a g e
m
D
No.
S
S
S
S
D
=1/N
=1/C*S
m
a
i
i
a
a,r (Sm=0)
1
30
5
15
15.52
2.0155E13
0
2
40
30
20
25.00
4.6303E11
0
3
30
45
15
21.43
7.9875E12
0
4
20
50
10
10.00
1.3461E15
0
5
50
45
25
25.00
4.6303E11
0
6
30
5
15
15.52
2.0155E13
0
7
100
20
50
57.69
6.3949E07
0
8
20
20
10
10.00
1.3461E15
0
9
30
25
15
15.00
1.3694E13
0
10
30
55
15
15.00
1.3694E13
0
170
5
85
87.93
7.8039E05
7.80E05
11
12
30
5
15
15.00
1.3694E13
0
13
30
5
15
15.00
1.3694E13
0
140
10
70
75.00
1.2729E05
1.27E05
14
190
5
15
95
98.28
0.00027732
0.000277
n
=15
D =
3.677E04
0.00036873
0
D=0.000370
D=3.677E04
L
= 1/D =2712.03
L
= 1/D =2719.61
R
R
N=n
*L
=15*2712.03=40680
N=n
*L
=15*2719.61=40794
0
R
0
R